Finite Element Analysis and Algorithms for Single-Crystal ... nr. 11-4.pdfFinite Element Analysis...
Embed Size (px)
Transcript of Finite Element Analysis and Algorithms for Single-Crystal ... nr. 11-4.pdfFinite Element Analysis...
INSTITUT FR WISSENSCHAFTLICHES RECHNEN UND MATHEMATISCHE MODELLBILDUNG
Finite Element Analysis and Algorithms for Single-Crystal Strain-Gradient Plasticity
B. D. Reddy C. Wieners B. Wohlmuth
Preprint Nr. 11/04
Anschriften der Verfasser:
Prof. B. D. ReddyCentre for Research in Computational and Applied MechanicsUniversity of Cape TownSouth Africa
Prof. Dr. Christian WienersInstitut fur Angewandte und Numerische MathematikKarlsruher Institut fur Technologie (KIT)D-76128 Karlsruhe
Prof. Dr. Barbara WohlmuthFakultat Mathematik M2Technische Universitat MunchenD-85386 Garching
FINITE ELEMENT ANALYSIS AND ALGORITHMS FOR
SINGLE-CRYSTAL STRAIN-GRADIENT PLASTICITY
B. D. REDDY, C. WIENERS , AND B. WOHLMUTH
Abstract. We provide optimal a priori estimates for nite element approximations of a model ofrate-independent single-crystal strain-gradient plasticity. The weak formulation of the problem takesthe form of a variational inequality in which the primary unknowns are the displacement and slipson the prescribed slip systems, as well as the back-stress associated with the vectorial microstress. Itis shown that the return mapping algorithm for local plasticity can be applied element-wise to thisnon-local setting. Some numerical examples illustrate characteristic features of the non-local model.
Key words. Strain-gradient plasticity, single crystal, rate-independent, a priori nite elementestimates, variational inequality, radial return algorithm
AMS subject classications. 65M12, 65M60, 65N22, 74H15, 74S05
1. Introduction. This work is concerned with the development and analysis ofnite element approximations and iterative solution algorithms of a model of small-deformation single-crystal strain-gradient plasticity. The model is assumed to berate-independent.
Strain-gradient theories of plasticity have been developed in response to the short-comings of classical theories of plasticity at the microstructural level. The classicaltheories lack a material length scale and are therefore unable to account for the sizeeects that are an important feature of behaviour in the range of tens to hundredsof microns. The inclusion of gradients of plastic strain in constitutive models allowsfor these size eects to be captured. Furthermore, when linked with the underlyingbehaviour of geometrically necessary dislocations, the continuum concept of plasticstrain gradients acquires a denite physical interpretation. Some representative worksin an extensive literature are those by Gudmundson, Fleck and Hutchinson, and Nixand Gao [13, 14, 15, 25, 29]. Examples of polycrystalline strain-gradient theory de-veloped within a thermodynamically consistent framework may be found in the worksby Gurtin and co-authors (see for example ) and Menzel and Steinmann .
Similar remarks apply to the development of theories of strain-gradient single-crystal plasticity, for which a number of models exist. These range from physicallymotivated theories due to Evers et al. and Bayley et al. [5, 6, 10, 11], to thoseby Gurtin and co-authors which are located within a thermodynamic framework,and which make use of the notion of microforces and microstresses which are power-conjugate to slip rates and their gradients, respectively (see [16, 17, 19, 21] and, for adetailed exposition, ).
With regard to computational approaches for single-crystal plasticity, relevantworks include those by Miehe and Schrder , Anand and Kothari , and Stein-mann and Stein . These works all deal with the rate-independent problem, whichis characterized by an algorithmic diculty: in the case of multiple slip systems theconstraints that dene yielding and ow on the dierent systems can be linearly de-
Centre for Research in Computational and Applied Mechanics, University of Cape Town, SouthAfrica. Email: firstname.lastname@example.orgInstitut fr Angewandte und Numerische Mathematik, KIT, Karlsruhe, Germany. Email:
email@example.comFakultt Mathematik M2, Technische Universitt Mnchen, Garching, Germany. Email:
pendent. The determination of active slip systems and solutions on these systemsthen requires the use of techniques such as generalized inverses and singular-valuedecomposition. In contrast, a number of computational studies in crystal plasticitymake provision for rate-dependent or viscoplastic behaviour, for which case the singu-larities associated with the linearly dependent systems do not arise (see, for example,Cuitio and Ortiz  and the aforementioned work by Evers et al. ). For the caseof strain-gradient plasticity Bittencourt et al.  have carried out a computationalstudy based on the model due to , with the aim of comparing continuum predic-tions with those obtained from discrete dislocation dynamics. They have treated therate-independent case, and consider examples of single-slip systems.
This work considers the theoretical analysis and numerical simulation of a rate-independent version, with non-zero hardening, of the model of non-local single-crystalplasticity due to Gurtin . The variational formulation of this problem has previ-ously been considered by Reddy , where the relationship between the defect energyand dissipation, and issues such as uniqueness of solutions, are explored.
The rst objective of the present contribution is to provide an analysis of thediscrete setting. A signicant feature of the discrete formulation is the introductionof the back-stress as an additional variable. An optimal a priori error estimate inspace is obtained for a single time-step nite element approximation of the problem.
The second contribution in this work relates to the use of a generalized Newtonmethod, which entails writing the set of equations and inequalities for the problemsas a set of nonlinear equations. The numerical examples presented in this work showthat the generalized Newton method provides an eective way around the linear de-pendence that causes diculties in the rate-independent problem. Nevertheless, thisapproach requires hardening in order to guarantee uniqueness in the local stress re-sponse.
The structure of the rest of this work is as follows. The model of strain-gradientcrystal plasticity and its variational formulation are presented in Section 2. Section 3is concerned with the introduction of discretization in space and time, while theoptimal error estimate is given in Section 4. The idea of the classical return mappingmotivates the formulation of a Newton-type algorithm in Section 5. Finally in Section6, numerical examples illustrate aspects of the algorithm and of the behaviour ofmulti-slip systems.
2. A model for gradient crystal plasticity. The governing equations for themodel of strain-gradient plasticity treated in this work are set out in this section.The approach follows that developed by Gurtin and co-authors in a series of works(see for example [17, 19] or the monograph ). In this section, the model underconsideration is presented without specifying the appropriate function spaces.
Let the reference conguration be a bounded Lipschitz domain in R3, and letDN = and HF = be non-overlapping decompositions of the boundary,where D and H are assumed to have positive measure. For simplicity of notation,only the case of homogeneous Dirichlet boundary conditions for the displacementson D is considered. The position of a material point is denoted by x and thedisplacement of the body from its reference conguration by u(x, t).
The displacement gradient u is decomposed additively into elastic and plasticparts he and hp respectively according to
u = he + hp . (2.1)
Small deformations are assumed so that the innitesimal strain is given by
= (u) = 12(u + (u)T
Plastic slip is assumed to take place on N planar slip systems, each having a unitnormal m and slip direction s on the th system. Here and henceforth lower-caseGreek indices run over 1 to N . A typical value is N = 12, for face-centred cubic(fcc) crystals. In special situations symmetry can be exploited, and the case N = 2is interesting to consider.
The plastic slip on the th plane is denoted by , and the plastic part of thedisplacement gradient is given in terms of the slip by
s m . (2.3)
This denes the elastic and plastic strain
e = e(u,) = (u) p() , p = p() = 12(hp + (hp)T
In (2.3) and hereafter, the notation denotes
N=1. Furthermore, the summation
convention is not assumed for Greek indices relating to slip systems.
The classical macroscopic equilibrium equation is given by
div + b = 0 in , (2.5a)
where is the Cauchy stress tensor and b the body force. The macroscopic boundaryconditions are
u = 0 on D , n = tN on N . (2.5b)
The microforce balance equation is given by
div + = 0 , (2.6a)
where the resolved shear stress on slip system is dened by
= s m .
In addition to this quantity, (2.6a) is expressed in terms of a scalar microforce
and a vectorial microstress . These two quantities are power-conjugate to the sliprate and its gradient , respectively. The boundary conditions associated with(2.6a) take the form
= 0 on H , n = 0 on F . (2.6b)
These are referred to respectively as micro-hard and micro-free conditions (see ).The free energy is assumed to take the form
(,,,) = e(, p()) + d() + h() (2.7)
in which and denote the arrays (1 . . . N ) and (1 . . . N ) of slips and hardeningparameters, respectively. The quantities e , d and h are respectively the elastic,